MULTI-SCALE ASSEMBLY METHODOLOGIES OF POLY(3- HEXYLTHIOPHENE) DERIVATIVE SYSTEMS FOR
ENHANCED OPTOELECTRONIC ANISOTROPY
A Thesis presented to
the Faculty of California Polytechnic State University, San Luis Obispo
In Partial Fulfillment
of the Requirements for the Degree
Master of Science in Polymers and Coatings Science
by David Bilger August 2017
© 2017 David Bilger
COMMITTEE MEMBERSHIP TITLE: AUTHOR: DATE SUBMITTED: COMMITTEE CHAIR: COMMITTEE MEMBER: COMMITTEE MEMBER:
Multi-Scale Assembly Methodologies of Poly(3-hexylthiophene) Derivative Systems for Enhanced Optoelectronic Anisotropy
Shanju Zhang, Ph.D.
Assistant Professor of Chemistry and Biochemistry
Chad Immoos, Ph.D.
Professor of Chemistry and Biochemistry
Erik Sapper, Ph.D.
Assistant Professor of Chemistry and Biochemistry
Multi-Scale Assembly Methodologies of Poly(3-hexylthiophene) Derivative Systems for Enhanced Optoelectronic Anisotropy
Conjugated polymers represent a class of semi-conducting materials with
numerous applications in optoelectronic devices, including organic light-emitting diodes, field-effect transistors, and photovoltaics. Because of the numerous advantages of macromolecular systems, including solution processing and
mechanical flexibility, conjugated polymers have become a burgeoning field of research with the hopes of producing cost-effective solution-based electronics.
Importantly, optoelectronic device performance is heavily influenced by conjugated polymer backbone orientation and overall thin film morphology. As such, the processing conditions of these systems are important to the construction of high-
performance optoelectronics. Polythiophenes are model conjugated polymers that have been studied extensively in halogenated organic solvents. However, the self-
assembly of these systems from dilute solution to the solid state remains ambiguous for solvents with high dielectric constants.
Here, two derivative compounds of poly(3-hexylthiophene) are
correspondingly investigated in high dielectric solvents by way of ultraviolet-visible absorption and fluorescence spectroscopy, Fourier transform infrared
solvent composition, and side-chain characteristics. The kinetics of these transitions are investigated, and a model is put forth to explain contrasting self- assembly mechanisms. At higher concentrations, both systems form lyotropic
liquid crystalline phases. Characteristics of the liquid crystalline phases are found to be heavily influenced by dilute solution self-assembly mechanisms and
processing. Through the application of a mechanical shear force along still-wet liquid crystal films, alignment of the polythiophene long axis is attained. This morphological characteristic is found to carry over to the solid-state for both
systems, and clear optoelectronic anisotropy of the thin films is observed. As such, these methodologies may provide a route to the production of environmentally
friendly high-performance optoelectronic devices.
Firstly, I would like to acknowledge and thank my advisor, Dr. Shanju Zhang. From the beginning, Dr. Zhang has provided both myself and my peers with every opportunity to be successful in our academic endeavors, whether
through research guidance, proposal writing, funding, or simple everyday advice. His determination to see his students succeed is second to none. I am lucky to
have worked with him, and I have become a much better individual for it.
Secondly, thank you to Dr.’s Sapper and Immoos for their involvement on my thesis committee, and with my academic career. Throughout my time at Cal
Poly, both of these individuals have made themselves available for discussion and advice, and have taken an active interest in my work.
Thirdly, I would like to thank all of those who have worked with me throughout my years at Cal Poly. Specifically, thank you to Amrita Sarkar and Dr. Morgan Stefik at South Carolina University, as well as Dr.’s Manesh Gopinadhan
and Chinedum Osuji at Yale University. The collaborative effort between Cal Poly and these institutions gave valuable insight into the chemical systems addressed
in this work. Additionally, thank you to my fellow peers, especially Jose Figueroa, Cameron Danesh, Greg Braggin, and Nathan Starkweather for their dedication, hard work, and insight with regards to the presented research.
Finally, thank you to Dr. Fernando and the Polymers and Coatings program, including all the professors associated with it. If not for my involvement with this
TABLE OF CONTENTS
LIST OF TABLES ……….. ix
LIST OF FIGURES ……… x
1. INTRODUCTION ……….. 1
1.1. History ……… 1
1.2. Conjugated Polymer Applications ……….. 3
1.3. Structure and Conductivity of Conjugated Polymers ………….. 8
1.4. Backbone Morphology of Conjugated Polymers ………. 12
1.5. Mechanisms of Polythiophene Self-Assembly ………. 16
1.6. Solution Processing of Conjugated Polymers ……….. 18
1.7. Multi-Scale Assembly Methodology of Conjugated Polymers ... 26
2. EXPERIMENTAL METHODS ……….. 28
2.1. Material Preparation ………. 28
2.1.1. System 1 ……… 28
2.1.2. System 2 ……… 30
2.2. Instrumental Methods of Characterization ……… 32
2.2.1. UV-Vis Spectroscopy and Spectrofluorimetry…………... 32
2.2.2. Small-Angle X-Ray Scattering ……… 35
2.2.3. Polarized Optical Microscopy ………. 38
2.2.4. Fourier-Transform Infrared Spectroscopy ……… 40
2.2.5. Four-Point Probe ……….. 40
3. RESULTS AND DISCUSSION ………... 44
3.1. System 1 ……… 44
3.1.1. Effect of Side-Chain Architecture and Length …………. 45
3.1.2. Time-Dependent Chromism ……… 52
3.1.3. Transition Kinetics ……… 55
3.1.4. Correlation Between ECL and Intrinsic Rigidity ……….. 59
3.1.5. Lyotropic Liquid Crystalline Self-Assembly ……….. 62
3.1.6. Electrical Properties of P3K6T-Surfactant Thin Films … 67
3.2. System 2 ……… 70
3.2.1. Dilute Solution Properties of P3CnTs ……… 70
3.2.2. Transition Kinetics of P3C5T ……….. 74
3.2.3. Liquid Crystal Gelation of P3C5T ……….. 79
3.2.4. Optoelectronic Anisotropy of P3C5T Thin Films ………. 85
3.3. Research Outlook and Future Work ……….. 88
4. CONCLUSIONS ……… 90
BIBLIOGRAPHY ……… 92
LIST OF TABLES
1. Calculated Persistence Lengths for P3K6T- STS16:DTS16
Supramolecular Complexes ……....………
LIST OF FIGURES
1. Chemical structures and nomenclature of notable semi-
2. Bar chart displaying the conductivity ranges that define
insulating, semi-conductive, and conductive materials …………...
3. Diagram depicting the major components of a photovoltaic layer stack. The active layer consists of both a donor and acceptor
4. Mechanism of charge separation in the active layer. (1) Light absorption leads to exciton formation in the donor material. (2)
Excitons diffuse to the donor/acceptor interface. (3) An electron transfers to the acceptor material. (4) An applied electric field separates the polaron pair. (5) The electron and hole are
transported to their respective electrodes12 ……… 5. (a) Ideal heterojunction morphology and (b) bulk heterojunction
6. Illustration of band gap energy levels in insulating, semi- conductive, and conductive materials ………
7. Chemical structure of polythiophene in its oxidatively, reductively, and non-doped states. Oxidative and reductive doping leads to the
formation of positive and negative quasiparticles, respectively19 ………... 8. The different directions of 2-D charge transport in organic semi-
conductors: Intermolecular charge hopping (top) and intramolecular backbone transport (bottom) ……….
9. A polythiophene chain with planarized segments (grey). The total length sum of the grey regions is the effective conjugation length of the chain24………..
10. Two step mechanism of the coil-to-rod transition in poly(3- alkylthiophenes)30.……….
11. Structural and morphological differences between crystalline solid, liquid crystalline, and isotropic states37………. 12. Characteristic phase diagrams of aqueous lyotropic surfactant
molecules. Below an appropriate temperature solid state crystals begin to form38 ………
13. Rod-like particles organized into (a) nematic, (b) smectic A, and (c) smectic C LC phases46 ……… 14. Photos and a schematic illustration of a two-step gelation process
of P3HT dissolved in o-xylene50……… 15. Model of CTAB complexed onto the backbone of PTEBS. (b)
Chemical structures of the surfactant (CTAB) and the polymer (PTEBS). (c) Depiction of hexagonal packing in the lyotropic LC
16. (a) Chemical structure of polythiophene P3KnT (system 1) with n = 4, 5, 6, or 7, (b) single-tailed surfactant (STSn) with n = 10, 12, 14, or 16, (c) double-tailed surfactant (DTSn) with n = 16, (d)
illustration of the supramolecular complexation of P3KnT with single and double- tailed surfactants, and (e) chemical structure of
polythiophene P3CnT (system 2) with n = 3, 4, 5, or 6 ……….. 17. (a) The working mechanism of a UV-vis spectrophotometer. Light passes through an entrance slit and monochromator. Upon
leaving the exit slit, monochromatic light passes through the sample and is transmitted to a detector. (b) Working mechanism
of a spectrofluorimeter63,64……… 18. (a) Concentration dependent UV-vis spectra of the 1:1
P3K6T:STS16 supramolecular complex at 50°C. (b) Calibration
curve of the 1:1 P3K6T:STS16 supramolecular complex ………….. 19. Transmission geometry SAXS. An imaginary vector connecting
the ends of the collimated and scattered X-ray beams represents the momentum transfer between incident and scattered light …... 20. (a) Optical image displaying a schlerien texture of the nematic LC
phase. (b) Working mechanism behind POM46,66………. 21. (a) Schematic of a four-probe configuration. Current is supplied
through the outer probes, and potential is measured by the inner probes. (b) Image of a four-point probe sample stage70………
22. FTIR spectra of pristine P3K6T and 1:1 P3K6T:STS16 supramolecular complex ………... 23. UV−vis spectra of dilute solution P3KnTs of varying alkyl-chain
length (n = 4, 5, 6, and 7) (a) before and (b) after complexation with STS16 over 90 min. The concentration of all solutions is 0.25
mM ………... 24. UV−vis spectra of (a) P3K6T complexed in 1:1 molar ratios with various single tailed surfactants STSn-1 and (b) with various ratios
of STS16: DTS16. The concentration of all solutions is 0.25 mM and the aging time is 90 min ……….
25. UV−vis spectra of (a) P3K6T complexed in 1:1 molar ratios with (a) various ratios of STS16:STS10 and (b) various ratios of STS16: STS14. The concentration of all solutions is 0.25 mM and the aging
time is 40 min ……….. 26. Images of aqueous 1:1 P3KnT:STS16 supramolecular complexes
at (top) 90 minutes and (bottom) two weeks after dissolution …….. 27. Time-dependent chromism of dilute solutions of the supramolecular complexes at 25 °C. (a) UV−vis and (b)
fluorescence spectra of 1:1 P3K6T:STS16;; (c) UV−vis and (d) fluorescence spectra of P3K6T-9:1 STS16: DTS16. The
concentration of all solutions is 0.25 mM ……… 28. Kinetics of the coil-to-rod transitions of diluted solutions of supramolecular complexes at 25 °C. (a) Time-dependent
absorbance at λ = 590 nm for 1:1 P3K6T:STS16, (b) the dependence of initial rate on polymer concentration for 1:1 P3K6T:STS16, (c) time-dependent absorbance at λ = 590 nm for
P3K6T-9:1 STS16:DTS16, and (d) the dependence of initial rate on polymer concentration for P3K6T-9:1 STS16:DTS16 …...
29. Concentrated kinetics of the coil-to-rod transition of supramolecular complexes at 25 °C. (a) Time-dependent absorbance at λ = 590 nm against aging time of 1:1 P3K6T:STS16,
(b) the dependence of initial rate on polymer concentration for 1:1 P3K6T:STS16.………...
30. Room temperature SAXS profiles of aqueous solutions of P3K6T
supramolecular complexes (∼0.60 wt %) with different
STS16:DTS16 ratios and pure P3K6T (∼0.20 wt %) ……….
31. Optical images of 51 wt % aqueous solutions of the 1:1 P3K6T-
STS16 supramolecular complex under crossed polarizers. (a) Without mechanical shearing and (b) with shearing. The arrow in part b indicates the shear direction ………..
32. Room-temperature liquid crystalline phase diagrams of P3K6T supramolecular complexes with (a) varying chain lengths of single
tailed surfactants (STSn-1) and (b) varying double tailed surfactant (DTS16) loading. Dashed lines guide the eyes only ………... 33. (a) Room temperature SAXS pattern and (b) temperature
P3K6T-STS16 supramolecular complex. The concentration of the
solution is ∼51 wt % ………
34. Optical images of a sheared LC film of P3K6T-STS16 complex under crossed polarizers after drying. (a) 0° rotation and (b) 45°
rotation. The arrows represent the shear direction ……… 35. Room-temperature measurements of anisotropic conductivity. (a)
Illustration of electrical conductivity measurements and (b)
current vs voltage curves of sheared P3K6T-STS16 LC films after complete drying parallel and perpendicular to the shear
direction……… 36. UV-vis spectra of dilute P3CnTs in DMSO with varied alkyl-chain lengths (n = 3, 4, 5, and 6) after 80-minute equilibration. The
concentration of solutions is 25 µg/mL ……… 37. UV-vis spectra (a) upon and (b) 24 hours after initial dissolution of P3C5T in varying ratios of DMSO:EtOH. The concentration of all
solutions is approximately 25 µg/mL ………... 38. UV-vis spectra of P3C5T thermochromism in (a) DMSO and (b) 8:2 DMSO:EtOH. The concentration of all solutions is
approximately 25 µg/mL ………... 39. Time-dependent chromism of dilute solutions of P3C5T in (a) DMSO and (b) 8:2 DMSO:EtOH. The concentration of all solutions
40. Assembly kinetics of diluted solutions of P3C5T at 25oC. (a) Time- dependent absorbance against aging time of P3C5T in DMSO, (b) the initial rate versus polymer concentration of P3C5T in DMSO,
(c) time-dependent absorbance against aging time of P3C5T in 8:2 DMSO:EtOH, and (d) the initial rate versus polymer
concentration of P3C5T in 8:2 DMSO:EtOH ……….. 41. FT-IR spectra showing the carbonyl shifting between P3C5T gels and solid films. The concentration of the gel is 30 wt% ……….
42. (a) Bulk and (b) thin film characteristics of concentrated P3C5T/DMSO thermoreversible gels. The concentration of all thin
films is 23 wt% ……… 43. Phase diagram of P3C5T in DMSO LC formation as a function of
concentration. Illustrative optical images of isotropic and liquid
crystalline phases are displayed above the phase boundary …….. 44. Optical images of periodic stripe textures of P3C5T in DMSO at
(a) 5x and (b) 10x magnification showing the periodicity of P3C5T banded textures ………... 45. Optical images of sheared films of gelled P3C5T in DMSO under
crossed polarizers. (a) 0° rotation and (b) 45° rotation of crossed polarizers. The solution concentration is 23 wt% and the shear direction is parallel to the single arrows ………..
46. (a) Optical images showing alterations of transmission intensity of sheared P3C5T films as a function of sample rotation. Plots of
Transmission intensity as a function of sample rotation in (b) Cartesian and (c) polar coordinates illustrating optical anisotropy of sheared P3C5T LC gel films. For both plots, normalization was
done over the entire range of data shown ………... 47. Room-temperature measurement of anisotropic conductivity. (a)
Current versus voltage curves of sheared P3C5T LC gel films after complete drying with probes parallel and perpendicular to the shear direction. (b) Bar graph comparing the anisotropic
conductivity of P3C5T LC gel films in parallel and perpendicular orientations relative to the direction of shear ………..
Polymeric materials have been employed extensively by human beings
over the course of our existence. In pre-historic times, these materials were exclusively bio-derived, mostly in the form of plant fibers, wood, bone, or skin.
Currently, polymers are not only derived from nature, but also by synthetic means. Despite our rich history with polymeric materials and their applications in everyday life, polymer science, from a molecular standpoint, is an advance with origins in
the twentieth century. The concept of macromolecules was first developed by Hermann Staudinger in the 1920’s1. Eventually, scientific inquires provided the
data necessary to prove Staudinger’s theories, and he was subsequently awarded the Chemistry Nobel Prize in 1953 “for his discoveries in the field of macromolecular chemistry”1. Eighteen years’ prior, Wallance Corothers invented
Nylon while undertaking research for DuPont2. The findings of Corothers demonstrated the significant potential of synthetic polymers on an industrial scale,
and not long after this did Karl Ziegler and Giulio Natta’s discoveries of polymerization catalysts shape the current polymers industry. In 1963, Ziegler and Natta jointly shared the Chemistry Nobel Prize “for their discoveries in the field of
the chemistry and technology of high polymers”3. Finally, Paul Flory provided the necessary theoretical explanations of macromolecular phenomena through his
fundamental achievements, both theoretical and experimental, in the physical chemistry of macromolecules”4.
While the works of Staudinger, Flory, Ziegler, and Natta provided numerous
advances to the field of polymer science, the specific materials investigated by these men consisted of saturated sp3 hybridized carbon backbones, resulting in
non-conductive properties. In 1977, Alan MacDiarmid, Hidekii Shirakawa, and Alan
Heeger experimented with non-saturated π-conjugated macromolecules, and were
successful in doping these materials over an extensive range of conductivities, from insulators to metals5. Prior to this, conjugated polymers were of little interest
due to their poor properties, including insolubility and minimal conductivity. As such, MacDiarmid, Shirakawa, and Heeger were jointly awarded the Chemistry
Nobel Prize in 2000, “for the discovery and development of electrically conductive polymers6.” This paved the way for new and exciting research at the interface of materials chemistry and condensed matter physics.
Shortly after the advent of conductive conjugated polymers, the study of such systems began expanding into many diverse fields. Notably, the inherent
connection between the charge transport and chemical structure of conjugated polymers began attracting the attention of synthetic chemists6. In the 1980’s, large
quantities of various π-conjugated macromolecules began being synthesized, and
processing capabilities of polymers. Accordingly, extensive efforts have been paid to characterizing these materials for use in numerous applications.
Figure 1. Chemical structures and nomenclature of notable semi-conducting
1.2. Conjugated Polymer Applications
Though various types of electronic devices exist in which conjugated polymers are applicable, including light-emitting diodes and field-effect transistors,
photovoltaic cells have become an exceedingly interdisciplinary and burgeoning field of research due to their numerous complexities. Currently, inorganic materials represent the industry standards with regards to photovoltaic devices8. This is due
exist between organic and inorganic conductors. First, charge carriers can move freely throughout the conjugated backbone of organic materials, but intermolecular transport through charge hopping is hindered8. This limits the charge transport
capabilities of organic materials compared to that of inorganic counterparts. Fortunately, organic materials possess large absorption coefficients, allowing for
the efficient capture of incoming photons9. Secondly, Frenkel excitons (electron- hole pairs) have been observed as the main charge carriers in organic materials, which makes electron extraction difficult in photovoltaic devices due to the strong
interactions between electrons and their respective holes8. In contrast, inorganic materials contain excitons of the Wannier-type, which allow for efficient separation
of electrons and holes due to binding energies that are on the same order as room temperature10. Despite these comparisons, inorganic electronics still retain numerous pit-falls with regards to processing, including expensive vapor
deposition techniques. Fortunately, where common inorganic materials have failed, conjugated polymers have the potential to succeed.
Figure 2. Bar chart displaying the conductivity ranges that define insulating, semi-
Because the electron transfer interactions between neighboring chains of conductive polymers are relatively strong compared to the intermolecular attractions of non-conjugated systems, conductive polymers tend to be insoluble.
Luckily, several chemical structures of conjugated systems have been synthesized with the capacity to mitigate solubility issues7. An example of this may be noted in
the structure of poly(3-alkylthiophenes) (P3AT), in which the incorporation of reasonably long side chains onto the thiophene monomer units allows for solubility in numerous organic solvents. As such, the capacity to produce electronic devices
of conducting polymers via solvent-based coatings processes, such as roll-to-roll printing, has become a distinct reality. Currently, two of the most high-throughput
methods for processing conductive polymers are flexographic printing and rotary screen printing11. While solution-based processing has been successful in producing electronic devices from conductive polymers, the average device
efficiencies are considerably low. As such, current research on conductive polymers seeks to increase electronic device efficiency while still maintaining cost-
effective solution-based processing.
The actual building of a polymer solar cell requires the construction of a layer stack, such as the one presented in Figure 3. After a conjugated polymer is
dissolved in an appropriate solvent, it is then transferred to a substrate through one of the aforementioned coatings processes. The necessary materials are
active layer consists of two sections, a donor and acceptor material, that act to effectively separate tightly bound Frenkel excitons8,12.
Figure 3. Diagram depicting the major components of a photovoltaic layer stack.
The active layer consists of both a donor and acceptor layer12,13.
The donor material (conjugated polymer) absorbs light and produces the bound
electron-hole pair, or exciton. Eventually, the exciton reaches the donor/acceptor material interface, and the electron is then extracted by the acceptor material. After extraction, the electron and hole each diffuse to their respective electrodes. If the
donor/acceptor interface is not reached within a few tens of nanometers, then the exciton will recombine and the solar cell efficiency will be suppressed14. An
illustrative description of this process may be seen in Figure 4. Therefore, the composition and arrangement of the layer stack, including the morphology of the active layer, can all have an effect on the overall photovoltaic device efficiency14.
As such, numerous techniques have been employed to improve device performance, and have ultimately led to device efficiencies of up to 10%15.
Figure 4. Mechanism of charge separation in the active layer. (1) Light absorption
leads to exciton formation in the donor material. (2) Excitons diffuse to the donor/acceptor interface. (3) An electron transfers to the acceptor material. (4) An applied electric field separates the polaron pair. (5) The electron and hole are
transported to their respective electrodes12.
In organic photovoltaics, the preferred active layer morphology is referred to as a bulk heterojunction, which is formed through the mixing of donor and acceptor materials. The ideal blended morphology entails a bi-continuous
interpenetration network, which is displayed in Figure 5a. In other words, domains of both donor and acceptor materials have sizes of twice the exciton diffusion
the bulk heterojunction is commonly referred to as a comb-like structure. Aside from controlling morphologies of the active layer, significant interest has been applied to tailoring morphologies of the individual donor and acceptor
materials14,16. This is particularly true of donor materials such as poly(3- hexylthiophene), in which more ordered crystalline arrangements have yielded
improved device efficiencies17. Notably, such an effect stems from the dependence of electronic character on the conjugated backbone arrangements of organic materials.
Figure 5. (a) Ideal heterojunction morphology and (b) bulk heterojunction
1.3. Structure and Conductivity of Conjugated Polymers
The mechanism of charge transport in organic macromolecules originates
from the existence of conjugated π bonds along the polymer backbone. This
alteration of adjacent double and single bonds produces polymers with continuous sp2 hybridized carbon centers. As such, one valence electron at each center
electrons to delocalize throughout the conjugated polymer main chain. However, in organic materials, the high binding energy of electrons makes them difficult to separate from their respective orbitals. The energy required to overcome the
potential barrier mentioned above is referred to as the band gap, and allows electrons to be excited from a valence band to a conduction band7. In organic
materials, the valence and conduction bands are referred to as the highest occupied molecular orbital (HOMO) and lowest unoccupied molecular orbital (LUMO), respectively7. The alteration of the band gap energy is what distinguishes
insulating, conducting, and semi-conducting materials, as shown in Figure 6. In inorganic conductors, the band gap is minimal to non-existent, and therefore
electrons may move freely in three dimensions due to the even spacing of molecular orbitals in all directions. In contrast, the continuity of conjugated polymers is variable, and the charge transport may be considered one
Figure 6. Illustration of band gap energy levels in insulating, semi-conductive, and
Due to the variable continuity and large binding energies of conjugated polymers, the materials exhibit inherent semi-conductive properties with increased band gaps compared to their inorganic counterparts. In order to mitigate these
properties, chemical doping of the conjugated polymer backbone is commonly employed to produce a net charge19. The charge may be either positive or negative
for oxidative or reductive doping, respectively. Halogens or alkali metals are commonly used to dope conjugated polymers;; as is the case with poly(3- dodecylthiophene), which sustains conductivities that approach 1000 S/cm when
doped with iodine20. While this value is still relatively small compared to a metal such as copper (5x105 S/cm), few applications of conjugated polymers require
conductivities greater than 1000 S/cm. The mechanism of how doping increases charge mobility results from interactions between opposing charges, which may be seen in Figure 7. For example, when a conjugated material is doped via
oxidation, an electron is removed from the backbone, producing a positive polaron. The positive polaron has strong interactions with the couter-ion of the
corresponding dopant. As such, localization and mobility of the polaron is strongly coupled to that of the dopant counterion. Therefore, increasing dopant concentration simultaneously increases polaron mobility and macroscopic
conductivity of the polymer. However, macroscopic charge-transport of conjugated polymers is dependent on multiple factors besides the dopant and dopant
Figure 7. Chemical structure of polythiophene in its oxidatively, reductively, and
non-doped states. Oxidative and reductive doping leads to the formation of positive and negative quasiparticles, respectively19.
From a quantum mechanical perspective, the band gap energy of conjugated polymers may be modeled as a particle that can move freely on an
infinitely thin wire. This model is appropriate as intra-chain charge transport is a one dimensional phenomenon. In such a model, the ends of the wire are
obstructed by infinitely large potential wells, and the potential energy of the free- moving particle along the wire is zero. For this system, solutions to the time- independent Schrodinger equation (after the application of boundary conditions)
indicate the particles wavefunction yields discrete energy levels. The energy eigenvalues of such a system may be calculated using equation 1
, 𝑤ℎ𝑒𝑟𝑒 𝑛 = 1, 2, 3 …(1)
where n is the energy level, ℏ is Plank’s constant divided by 2π, me is the mass of
an electron, and L is the length of the infinitely thin wire. In principle, the energies of the HOMO and LUMO energy levels may be calculated using equation 1, and the absolute difference between them will yield a theoretical value of the band gap.
Intriguingly, the relationship presented in equation 1 implies that the length of the wire directly effects the HOMO and LUMO energy levels, and therefore the band
gap. Since electrons of conjugated polymers delocalize through pz orbitals of the main chain, conjugation length is analogous to the theoretical wire length. Therefore, promoting orbital overlap by controlling the backbone morphology of
conjugated polymers represents an alternative method by which to influence the band gap energy.
1.4. Backbone Morphology of Conjugated Polymers
While chemical doping and the model of a particle on an infinitely thin wire
both improve and explain charge transport of conjugated polymers within an individual chain (intra-chain transport), electrons may also move perpendicularly
between separate chains (inter-chain transport)21. In the ideal case, conjugated polymers may be thought of as perfectly rigid and linear conductive wires, with of intra-chain charge transport relative to inter-chain charge hopping. In this scenario
However, from an applications perspective this ideal example is ultimately impractical. To work effectively, the length of the individual polymer chains would have to span the entire structure of a device, which has never been achieved.
Consequently, macroscopic conductivity over long distances in bulk conjugated polymers is dependent on inter-chain mechanisms. Unfortunately, such
mechanisms are greatly hindered by alignment defects along individual polymer main chains22. These imperfections introduce charge traps into the conjugated backbone, and suppress two dimensional conductivities. Importantly, these
defects may be diminished by the appropriate control of conjugated polymer microstructure and crystallinity, allowing for augmented two dimensional mobility
of charge carriers through intra and inter-chain transport.
Figure 8. The different directions of 2-D charge transport in organic semi-
conductors: Intermolecular charge hopping (top) and intramolecular backbone transport (bottom).
Control of crystalline morphologies in conjugated polymers, namely poly(3- hexylthiophene) (P3HT), have been demonstrated to enhance the performance of photovoltaic devices23. Kinks and bends along the conjugated polymer backbone
act to effectively increase the systems band gap. However, promotion of crystalline regions between backbones leads to more rigid and ordered structures, which
correspondingly results in the geometrical alignment of pz orbitals. As discussed previously, the infinitely thin wire model shows that alignment of pz orbitals increases the conjugation length, and reduces the band gap energy. However, as
polymers never exist as completely crystalline materials, conjugation is not continuous, but instead exists in rather discrete regions. The ensemble average of
such regions has therefore been deemed as the effective conjugation length, and correlates well with overall chain rigidity and crystallinity.
Figure 9. A polythiophene chain with planarized segments (grey). The total length
sum of the grey regions is the effective conjugation length of the chain24.
P3ATs are well studied systems due to their reduced band gaps and impressive charge carrier mobility25,26. Additionally, P3ATs have large ionization potentials (~ 5 eV) that prevent oxidation under ambient conditions, imparting
stability for photovoltaic device applications27. This is in opposition to highly conductive organic counterparts, such as polyacetylene, which oxidizes readily
under ambient environments. The most studied of the P3AT family is P3HT, which has an effective conjugation length that is directly related to its backbone orientation and morphology. While numerous factors can affect these orientations,
investigations of how solvent choice influences P3HT crystallinity are ubiquitous throughout the literature28,29. In P3HT, solution-based self organization forces the
thiophene monomer units to align in anti-coplanar arrangements. These orientations result from solvent interactions with the polymer backbone that eventually lead to an equilibrium conformation. In a good solvent, the polymer
backbone is highly solvated, and exists in a stable coil-like conformation. In contrast, poor solvents introduce thermodynamic instability into the system, and
backbone conformation is altered to achieve a more stable state. Rod-like conformations are thus promoted due to their lower resonance energy and delocalization tendencies30. As such, the rod-like conformation of P3HT enhances
the backbone planarity and effective conjugation length. The formation of backbone planarity is commonly accompanied by the presence of rod-like
aggregates30. Intriguingly, intermolecular forces between polymer chains,
especially π-π stacking interactions between pz orbitals of the thiophene rings, are
interactions that arbitrate solid-state crystal formation. Yet, dried films of P3HT aggregates lack long range order and are inhomogeneous, providing an additional barrier to enhancing conductivity. Furthermore, solvent choice also plays a
significant role in coatings processes for roll-to-roll printing. Properties such as solution rheology, film thickness, ambient vapor pressure, and environmental
impact must all be considered. Thus a delicate balance between the latter properties, P3HT solubility, and crystal formation should be achieved through careful solvent selection.
1.5. Mechanisms of Polythiophene Self-Assembly
From a mechanistic point of view, the relationship between chain alignment and intermolecular aggregation is a chicken or the egg scenario. That is, do individual polymer chains align and subsequently aggregate, or does aggregation
force chain planarization? In the latter case, intermolecular aggregation of multiple chain segments is a single step mechanism that leads to fringed micelle-like
structures32. As the chains come together, forced planarization of the polythiophene backbone is induced. In contrast, the latter mechanism calls for individual polythiophene chains to undergo intramolecular reorganizations from
coil-like to rod-like conformations32. These rod-like chain segments subsequently aggregate following backbone reorganization. As such, the intramolecular coil-to-
conjugated polymer self-organizations has been heavily debated for multiple systems, including polydiacetylenes and polythiophenes.
Figure 10. Two step mechanism of the coil-to-rod transition in poly(3-
It is understood that the self-organization mechanism of P3AT assembly results from a coil-to-rod conformational transition, which may be of inter- or intamolecular origin to form aggregates of nanofibrils. Structurally, such nanofibrils
are upheld through the formation of hairpin-like lamella that propagate through the back and forth folding of polymer chains. As mentioned previously, some believe
the coil-to-rod transition to be the primary driver for self-assembly, while others insist rod-rod aggregation dominates. Previous reports have shown the solution assembly kinetics of P3HT in a marginal solvent to be of a mixed fractional order,
possible to explain the growth rates of numerous P3AT systems by the total individual contributions of nucleation (Si) from various physical processes35. It can then be stated that the total nucleation of P3ATs will result from differing influences
of the following components in equation 2
𝑆898:; = 𝑊=𝑆= = 𝑊>9=;𝑆>9=;+ 𝑊@9;A𝑆@9;A+ 𝑊:BBCDB𝑆:BBCDB (2)
where Wi is the weighting factor determining the intrinsic contribution of each term.
Additionally, each contributor has a fundamental scaling relationship associated with the physical process it represents. For instance, the chain folding process has
previously revealed kinetics of a fractional order, similar to those reported for P3HT in a marginal solvent. However, controlling the weighting factors associated with the coil-to-rod and aggregation processes has yet to be explained unambiguously
for polythiophene systems. Moreover, control of such self-assembly mechanisms may allow for the optimization of solid-state morphologies and processing
1.6. Solution Processing of Conjugated Polymers
Liquid crystals (LC) represent a specific phase of matter that lies at the nexus of solids and liquids. As the name implies, LCs maintain an overall ordered
conjugated polymers, lyotropic processing has become an immense interest as it possesses the potential to produce macroscopically ordered thin films.
Figure 11. Structural and morphological differences between crystalline solid,
liquid crystalline, and isotropic states37.
Lyotropic LCs were first investigated in aqueous systems of surfactant
molecules36. Above the critical micelle concentration (CMC), self-organization of free surfactants into organized micelles becomes thermodynamically favorable. As concentration increases, the surfactant molecules pack into various shapes,
Figure 12. Characteristic phase diagrams of aqueous lyotropic surfactant
molecules. Below an appropriate temperature solid state crystals begin to form38.
It was not until scientists at DuPont formed lyotropic LCs of the well known
polyaramid, Kevlar, that solution processing of polymeric materials began gaining momentum. By using a combination of intermolecular hydrogen bonding and
shear-induced alignment, films and fibers produced from Kevlar yielded exceedingly high tensile strengths39. Since that time, it has been realized that the long range order inherent in LC materials may be promoted to the solid state. In
the case of conjugated polymers, solution-based self-assembly of lyotropic LCs has been shown to produce thin films with an increase in conductivity by three
shown promise in improving optoelectronic device effeciencies41–43. On the basis of Onsager’s rigid-rod model, the promotion of smectic and nematic LC phases is driven through the presence of rigid, high aspect ratio microstructures44. As the
concentration of a rod-like particle solution increases, a rotational component of entropy is minimized. To counteract this effect, adjacent rod-like particles pack
more efficiently to exclude solvent volume, increasing the overall entropy of the system and forming the LC phase. In this way, ordered LC domains that span over hundreds of micrometers may be promoted in thin-films constructed from dilute
rod-like particle solutions. Moreover, alignment of LC domains that span even greater length scales may be achieved through external influences, such as
mechanical shearing (as was the case with Kevlar), electric, or magnetics fields40,45.
Figure 13. Rod-like particles organized into (a) nematic, (b) smectic A, and (c)
smectic C LC phases46.
In addition to achieving long range order in conjugated polymer thin films, the presence of an interconnected network structure is highly desirable for photovoltaic applications47,48. However, this goal is difficult to achieve when the
processing conditions of conjugated systems highly influence structural development. Because of this, self-assembly prior to film deposition can help
ensure the formation of a desirable three dimensional network structure. Such a configuration can be obtained through the formation of a gel, which is a material with subunits that bond to form a network. Bonds linking the subunits can either be
formed through covalent means, indicating the gel is permanent, or through intermolecular interaction, leading to thermoreversibility. Importantly, gelation of
conjugated polymers in organic solvents is a common phenomenon, and the formation of P3AT organogel systems have been widely reported in the literature49. Interestingly, polymer entanglement helps to foster the formation of crystalline
nanofibrils, which can then promote the construction of an interconnected 3-D network.
Figure 14. Photos and a schematic illustration of a two-step gelation process of
Malik et al. demonstrated that interconnected fiber networks present in P3HT gels led to higher charge mobility compared to traditionally produced films from spin- casting51. While the elastic nature of gels makes them difficult to process through
many traditional coatings techniques, recent efforts have demonstrated the feasibility of using conjugated polymer organogels in the processing of photovoltaic
devices, including the formation of microgel particles, freeze-drying methods, and organogel sonication47. Additionally, non-halogenated/low volatility solvents have been used to control P3AT gelation while allowing for the formation of uniform thin-
film gels under ambient conditions52.
While the solution processing of conjugated polymer thin films provides
strict advantages in the production of optoelectronic devices over costly inorganic- based counterparts, it also introduces its own set of concerns. The use of halogenated solvents, including chloroform, chlorobenzene, and dichlorobenzene
are often utilized to mitigate issues observed in the film forming process of conjugated polymers53. However, solvents such as these are harmful to human
health and yield a high energy cost due to their toxicity and environmental impact54. Such properties lend these solvents to being unsustainable, and stricter regulations on the mass production of these chemicals only makes the processing
of conjugated polymers less promising. As such, further efforts have been focused towards achieving environmentally friendly methodologies for the processing of
friendly means. This is most likely a result of the delicate interplay between polymer morphology, solvent composition, and photovoltaic device performance. Therefore, any change in the polymer nanomorphology will result in a change in
device performance. This means new understandings between the interplay of nanomorphology and device performance must be established for conjugated
polymer systems consisting of benign solvents and new functionalities.
In order to facilitate the processing of conjugated polymers in more polar solvent systems, modifications to structure and side-chain functionality have been
synthetically employed. This typically calls for the incorporation of charged polar groups along the backbones of conjugated polymers, resulting in so called
conjugated polyelectrolytes. The inclusion of such new functionalities along the conjugated polymer backbone also leads to water solubility, providing a probable pathway to environmentally friendly solution processing57. However, conjugated
polyelectrolyte films constructed from aqueous solutions lack the crystalline characteristics necessary to enhance photovoltaic device performance. This is the
result of aggregate formation in aqueous solutions of conjugated polyelectrolytes. The coloumbic repulsion of the ionic side-chains leads to backbone interactions
through π-π stacking, which prevents hydrophobic regions of the polymer chains
from interacting with the surrounding aqueous medium58. Because of this issue,
researchers have focused their attentions on tailoring the morphology of conjugated polyelectrolytes in aqueous media.
aggregation 57,58. While both ionic and neutral surfactants have been utilized, the use of counterionic surfactants have been shown to result in the formation of supramolecular complexes. This is due to coulombic attraction between charges
of the conjugated polyelectrolyte side-chains and surfactant molecules. Interestingly, the formation of lyotropic liquid crystals have been reported in
aqueous solutions of the surfactant centyltrimethylammonium bromide complexed with a conjugated polyelectrolyte derivative of polythiophene in 1:1 molar ratios59. Further analysis by small-angle X-ray scattering suggested that the
supramolecular complexes formed hexagonal microstructures above a critical solution concentration. The self-assembly of such microstructures may provide a
suitable methodology for the control of conjugated polyelectrolyte morphology in aqueous media.
Figure 15. (a) Model of CTAB complexed onto the backbone of PTEBS. (b)
Chemical structures of the surfactant (CTAB) and the polymer (PTEBS). (c) Depiction of hexagonal packing in the lyotropic LC phase59.
Aside from the incorporation of electrolytes onto the backbone structure of polythiophenes, functional groups that allow for short-range interactions between thiophene units have also been produced60,61. One such common functionality is
that of a carboxylic acid, or any other group which has the potential to act as both a hydrogen bond donor and acceptor. In contrast to the repulsive forces of
similarly charged side-chains, hydrogen bonding allows for attraction between polymer chains, promoting thermorevesible linking between adjacent monomer units. Such interactions have been found to assist in the processing conditions
conjugated polymers, and even result in the formation of gels62. These intermolecular cross-links incorporate plasticity into the polymer gel, and allow for
ease of alignment processes. As such, the investigation of polythiophene derivatives with the potential to hydrogen bond may provide interesting processing alternatives compares to polythiophene-based CPEs.
1.7. Multi-Scale Assembly Methodology of Conjugated Polymers
When using a multi-scale assembly approach, modifications to the conjugated polymer system (surfactant addition, poor-solvent addition, etc.) are made in the dilute regime. Such adjustments are done with the intention of
promoting high aspect ratio microstructures through the coil-to-rod transition. By raising concentrations of the rod-like particle solutions past a critical value, the
films are produced that sustain significant optoelectronic anisotropy in the solid state.
In this work, enhanced anisotropy of poly(3-hexylthiophene) derivative thin
films was achieved for two separate systems using a multi-scale assembly methodology. In the first system, carboxylate functionalized P3HT is ionically
bonded with aqueous quaternary ammonium surfactants in 1:1 molar ratios to form a supramolecular charge-neutral complex. For the second system, carboxylic acid functionalized P3HT is dissolved in various ratios of dimethyl sulfoxide and
ethanol. In dilute solutions of systems 1 and 2, the coil-to-rod transition is investigated as a function of surfactant architecture and solvent composition,
respectively. The origin of the coil-to-rod mechanism is revealed for both systems through transition kinetics. In concentrated solutions, both systems under-go isotropic to LC phase transitions. Interestingly, system 2 forms an LC gel in
contrast to system 1. The mechanism of the coil-to-rod transition is believed to play a role in the resulting LC gelation. The application of a mechanical shear force
aligns the LC samples of both systems, and a significant optoelectronic anisotropy is observed in the dried thin films.
2. Experimental Methods 2.1. Material Preparation 2.1.1. System 1
Regioregular (82−90% head-to-tail) poly[3-(potassium- 4- butanoatethiophene)-2,5-diyl] (P3K4T, average Mw = 14 kg/mol, Rieke Metals
Inc.), poly[3-(potassium-5-penanoatethiophene)-2,5- diyl] (P3K5T, average Mw = 35 kg/mol, Rieke Metals Inc.), poly[3-(potassium-6-hexanoatethiophene)-2,5-diyl] (P3K6T, average Mw = 60 kg/mol, Rieke Metals Inc.), poly[3-(potassium-7-
heptanoatethio- phene)-2,5-diyl] (P3K7T, average Mw = 60 kg/mol, Rieke Metals Inc.), centyltrimethylammonium bromide (Sigma-Aldrich) including its various alkyl
chain derivatives with the side-chain length equal to 10, 12, and 14 carbons, and dihexadecyl dimethylammonium bromide (Sigma-Aldrich) were used as received in preparation of stock hydrogels (0.10 M). Initially, individual polymer and
surfactant solutions were prepared in 1:1 molar ratios at concentrations of 0.20 M in plastic microcentrifuge tubes. All solutions were made with nanopure water
(Milli-Q, 18 MΩ). After dissolution, individual polymer and surfactant solutions were sonicated for 20 minutes at a temperature of 60°C. The samples were then heated in a temperature controlled oil bath at 70°C for 1 hour or until fluid. While still in the
oil bath, solutions were transferred by dropwise addition of surfactant to polymer, resulting in supramolecularly complexed samples with concentrations of 0.10 M.
Centrifuge Biotechnical Services Inc.) for 30 min at a speed of 10,000 rpm, resulting in stable hydrogels. Little to no phase separation was noticed after centrifugation. The chemical structures and nomenclature of both polymers and
surfactants are shown in Figure 16.
Figure 16. (a) Chemical structure of polythiophene P3KnT (system 1) with n = 4,
5, 6, or 7, (b) single-tailed surfactant (STSn) with n = 10, 12, 14, or 16, (c) double- tailed surfactant (DTSn) with n = 16, (d) illustration of the supramolecular
complexation of P3KnT with single and double- tailed surfactants, and (e) chemical structure of polythiophene P3CnT (system 2) with n = 3, 4, 5, or 6.